# RSC Article Template (PC)

## Сomentários

## Transcrição

RSC Article Template (PC)

CREATED USING THE RSC ARTICLE TEMPLATE - SEE HTTP://WWW.RSC.ORG/IS/JOURNALS/TEMPLATES/TEMPLATES.HTM FOR FURTHER DETAILS Calculations of Optical Properties of the Tetraphenyl-X Family of Isomorphous Crystals (X=C, Si, Ge, Sn, Pb) Kacey Claborn, Bart Kahr* and Werner Kaminsky† Department of Chemistry, Box 351700, University of Washington, Seattle, WA 98105, USA * [email protected], † [email protected] This submission was created using the RSC Article Template (DO NOT DELETE THIS TEXT) (LINE INCLUDED FOR SPACING ONLY - DO NOT DELETE THIS TEXT) As part of a program to determine how small structural changes become manifest in the optical properties of crystals we used classical dipole-dipole interaction calculations to estimate the linear birefringence and optical rotatory power of the crystals Ph4X where X=C, Si, Ge, Sn, and Pb. Field induced effects including second harmonic generation, the electro-optic response and electrogyration were calculated using the dipole electron shifting model (DES) model. The calculated induced effects are larger than those in standard materials such as KH2PO4. All of the properties tend to increase in magnitude with increasing polarizability except for optical rotation, which is largest for Ph4C. We propose an interpretation for the unusual behaviour of the optical rotation in terms of competing helical circuits of closely bonded atoms. Introduction where Z is the Hertz vector potential. The term in braces has the periodicity of the lattice. The overall Hertz potential is built from terms describing the frequency dependent incident wave, the interaction between all atoms in the unit cell and the interaction between all unit cells in the lattice, respectively. The electric field E(rsl) at atom rsl originating from the dipole waves emanating from all other atoms (point dipoles) in the structure is described by (Figure 1):3 Tetraphenylmethane crystals belong to a family including the isomorphous tetraphenyl derivatives of silicon, germanium, tin and lead. This is a rare family of molecular crystals whereby a main group element in the 2nd row can be replaced by any other atom in the corresponding family, group 14 in this case, without changing the essential features of the crystal structure. As crystal engineers aspire to understand the effects of small prescribed structural changes on the physical properties of crystals, the isomorphous family, Ph4X where X = C, Si, Ge, Sn and Pb, provides unparalleled opportunities for comparison. Here, we present classical calculations of the optical properties of the Ph4X family including linear birefringence, optical rotation, as well as second harmonic generation (SHG), the electro-optic effect and induced optical rotation (electrogyration), non-linear optical effects that are of great interest to many scientists in the crystal engineering community. The parameterization of these calculations is based on redetermined experimental values of refractive indices that are at great variance with those previously reported. E(rsl ) = grad divV − ∂ 2V = ∑ Ass ' p ls ' = α s−1p ls c 2 ∂t 2 s' where psl is the electronic polarization at position rsl and αs is the electronic polarizability volume of atom s. Ass´ is a matrix of complex numbers. Computation Methodology Dipole-Dipole Interaction Optical rotation may be calculated using the dipole-dipole interaction theory and has been applied with success to This theory based on electronic ionic crystals.1 polarizabilities is described elsewhere.2 Here, we outline the basic ideas behind the calculations. Polarizability volumes were selected so that the dipole-dipole model calculations were close to the refractive indices derived experimentally. The cumulative effect of the dipole-dipole interactions between all atoms in the crystal lattice acting on an atom s in unit cell l at a position rsl is described by an electrical potential, V:2 V = Z ls'' (rsl ) = [ ( exp ik o rsl − rsl'' − ik rsl − rsl'' exp(−iωt )∑ p s ' exp(ikrsl )∑ ' 4πε o rsl − rsl'' s' l ' Figure 1. Illustration of the dipole-dipole interaction theory of Devarajan and Glazer (1986). When an initial wave with polarization E passes the first atom positioned at (x,0,0) in a Cartesian reference system (z//k, k is the wave vector), a dipole field is created which induces in a second atom at (0,y,z) a secondary dipole field. This field oscillates in a direction different to E for y, z ≠ 0. The interference of all induced waves with the initial wave (calculated via an Ewald sum) on passing through the crystal leads to a rotation of E when at least four atoms adopt a chiral arrangement. The result is a conversion of the atomic polarizabilities from an isotropic to an anisotropic state. The imaginary part contained therein describes the phase shifts that result in radiative interference and optical rotation. When the sum of the contributions to the electric field is then taken the series converges only conditionally. As a remedy, the function is decomposed into a Fourier series that can be separated into two )] 1 CREATED USING THE RSC ARTICLE TEMPLATE - SEE HTTP://WWW.RSC.ORG/IS/JOURNALS/TEMPLATES/TEMPLATES.HTM FOR FURTHER DETAILS absolutely convergent parts, one in real space and the other in reciprocal space according to the Ewald theorem.4 A new matrix Css´ is defined from variables describing the electric field E(rsl): ( C ss ' = (α s−1δ ss ' − Ass ' + const ) −1 = α S−1δ SS ' − QSS ' where a spherical depolarization field (Lorentzdepolarization) is assumed. The largest approximation in the DES model is the substitution of the ionic polarizability, which should be used to calculate the shifts x for static electric fields, by the electronic polarizability volumes. The ionic polarizabilities are not well known, in contrast to the electronic polarizabilities, which are derived from refractive indices and which are tabulated elsewhere.9 Naturally, atoms with small electronic polarizabilities are only slightly affected by a static electric field.10 Furthermore, if the sum of the molar polarizabilities is increased only by about a factor of three, the dielectric constant tends already to infinity, as is easily seen from the Clausius-Mosotti relation. Thus we can expect only a relatively small error by this approximation as long as the dielectric constant remains small. This is not the case when a crystal is ferroelectric, or has field dependent internal dynamics. It is of particular interest, therefore, to see if this crude approximation can be justified in the Ph4X family. ) −1 The imaginary part of this matrix is related to optical rotation. For the calculation of Qss´ see Appendix 1. The optical rotation ρ(k) and optical dielectric constants εij are derived as follows:1 ρ (k ) = −erij k r 2nv ε ij = δ ij + 1 ν Im ∑ (C ss ' ) ij ∑ (C ss ' ss ' ) ij ss ' (erij = Levi-Civita symbol, k = wave vector, n = average refractive indices, v = unit volume and δij = Kronecker delta). The Levi-Civita operation erij accomplishes the cross product between the spatial coordinates of Css′ and the wave vector.The dipole-dipole interaction distorts the polarizabilities of the atoms resulting in an anisotropy described by the effective polarizabilities αseff: α seff = Re ∑ C ss ' s' This theoretical model reliably calculates optical rotation on the basis of the interacting forces in inorganic structures. It was further applied successfully to molecular crystals where the interacting fields within a molecule are more significant than those between the molecules.5,6 Here, we are trying to evaluate the applicability of the classical theory to aromatic molecular crystals, even though we have explicitly neglected the electronic structure of the molecules in our calculations. While progress has been made in the application of quantum mechanics to the calculation of optical rotation in molecules7, in crystals we chose a theory that embodies long range interactions and accommodates the periodicity. Figure 2 The shift of the nuclei relative to the electron clouds by an external electric field E. The radius of the clouds indicates the size of the polarizability. The external field induces a small change in the value of the electronic polarizability volumes, but this effect is neglected in the DES model. Furthermore, in the hard-spheres approximation, the electronic clouds of different atoms are not free to move relative to each other. In a classical picture at optical frequencies, the atom’s nucleus is the center of the light-wave induced vibration of the shell. Dipole Electron Shifting (DES) The dipole-dipole theory was used to calculate the rotatory power ρij (o/mm) and the optical relative dielectric constant εij with and without the applied field. The polarization tensor aij is the inverse of εij: aij=εij-1,11 n is the average refractive index and λ is the wavelength. The dispersion of αij is roughly approximated by a λ-1/2 dependence for the SHG calculations. These quantities as well as the electrogyration gijk and linear electro-optic effect at constant strain rijk were calculated from the following equations: To calculate the higher order optical properties, the classical polarizability theory was employed according to the procedure of Kaminsky and Glazer, whereby a virtual external electric field displaces the nuclei from the centers of the surrounding electron clouds in proportion to the atomic electronic polarizabilities.5 In the DES model, the external electric field shifts the atomic nuclei by distance x in proportion to the polarizability of the kth atom (Figure 2): 8 xi (k ) = ρij(Ekexternal) - ρij(0) = gijkEkexternal/nλ (electrogyration at 4πε 0 α ij (k ) E loc j e aij(Ekexternal) - aij(0) = rijk Ekexternal εij(Eklight) - εij(0) e is the charge of an electron, εo is the permittivity of free space and Ejloc is the local electric field connected with the external field Eext via the effective relative dielectric constant ε' in the direction of the external field: E loc = = 2dijkEklight constant strain) (electro-optic effect at constant strain) (second harmonic generation). The rotatory power ρij is defined as the clockwise rotation of linear polarized light passing through a non-birefringent sample of 1mm thickness as observed when looking towards the light source. The tensor symmetry (dijk = dikj) was applied artificially to the calculated d-coefficients. Since εij=εji, the resultant dijk was totally symmetric, as expected for transparent crystals (Kleinmann’s rule).12 All (ε '+2) ext E 3 2 CREATED USING THE RSC ARTICLE TEMPLATE - SEE HTTP://WWW.RSC.ORG/IS/JOURNALS/TEMPLATES/TEMPLATES.HTM FOR FURTHER DETAILS negative optical character throughout the series.15 The experimentally determined linear birefringence showed a strong variation that is correlated with the polarizability of the central atom. other tensors were calculated assuming no symmetry at all. Therefore, it was satisfying to discover that the resulting tensors conform to Neumann’s law. Experimental Curiously, Newkirk reported that the refractive indices for all the crystals in the Ph4X family were essentially the same at 1.58±0.05, and that the crystals were all uniaxial positive.16 Both statements are incorrect. Our results are reliable within 0.01 of the absolute values and the difference between largest and smallest refractive index is 0.39. Crystal Growth The tetraphenyl derivatives of carbon, germanium, tin and lead were obtained from Aldrich and crystals were grown by slow evaporation from saturated solutions of chloroform in a water bath at 30°C. Crystals of tetraphenylsilane grown from the melt were donated by Prof. S. Haussühl (Cologne, Germany). Results of Calculations and Discussion X-Ray Difraction Analysis For all calculations, one needs the x-ray structure coordinates as well as the absolute refractive indices as reference. The polarizability volumes αH for hydrogen atoms and αC for carbon atoms were chosen to best match the experimental optical character. The values of αX were chosen to best match the experimental average refractive indices. In Ph4Si and Ph4Ge we could not simultaneously match the absolute value of the refractive indices and the experimental optical character. We then sacrificed the optical character, which is less important than the absolute values. The resulting estimation of optical properties is shown in Table 2 and the corresponding tensor surfaces in Figure 4. For internal consistency x-ray crystal structures of all of the members of the Ph4X family were redetermined13 with a Nonius Kappa CCD diffractometer. Data were refined to R=2-5%. All measurements were carried out at room temperature. The hydrogen atoms on Ph4Pb were placed using a riding model. Lloyd and Brock recently presented a detailed comparative analysis of these crystal structures.14 The tetraphenyl family crystallizes in the tetragonal space group P 421c (D2d) and the molecules sit on the improper fourfold axes. In this point group there is only one independent gyration tensor element, g11 = -g22 just as for KH2PO4 and its isomorphs.† Refractive Index Determination Table 2 Calculated optical properties at 670nm (d-coefficients at 1064nm) and structural details. αC (phenyl) = 0.580Å3, αH = 0.058Å3. β: angle between adjacent phenyl groups (see Figure 6); γ: dihedral angle between phenyl rings. Refractive indices were determined (Table 1) using a micron scale microscope and the three height method derived from Snell’s law of refraction (Figure 3). This 'old-fashioned' method was more reliable than the prism The method because Ph4X crystals polish poorly. birefringence measurement was refined using standard methods of polarized light microscopy confirming X= C αX(Å ) 3 0.62 ne 1.425 no 1.455 252 ρ11 (°/mm) -0.030 d123 (10-12m/V) d312 (10-12m/V) -0.034 -1 ε r123 (10-12m/V) -0.273 1.42 ε-1r231 (10-12m/V) -0.14 ε-1g231 (10-5 º/V) 106.8 β (º) 74.8 γ (º) 32.0 β-γ (º) X-C2 (Å) 1.5491 a (Å) 10.9050 c (Å) 7.2850 Si Ge Sn Pb 4.50 1.755 1.667 32 -0.094 -0.89 5.8 7.7 -0.92 108.0 80.6 28.4 1.8730 11.4448 7.0640 5.00 1.649 1.608 -33 -0.094 -0.88 3.5 4.7 -0.30 108.4 83.6 24.8 1.9517 11.6160 6.9020 8.80 1.824 1.833 -75 -2.57 -2.47 9.2 11.0 -1.75 110.9 88.9 22.0 2.1430 12.0680 6.5570 9.50 1.747 1.767 -40 -2.58 -2.39 9.2 9.5 -1.87 111.1 87.6 22.5 2.2225 12.1110 6.5430 Figure 3 Experimental determination of absolute refractive indices using the 3-height method: n sin α tan α d L2 L1 h3 − h1 = ≈ = = = nair sin β tan β d L1 L2 h3 − h2 where nair is assumed to be one. Table 1 Experimental refractive indices in Ph4X at 650nm. Reliability of absolute refractive indices is ca. ±0.01. X= C Si Ge Sn Pb ne no ∆n 1.446 1.476 0.030 1.706 1.742 0.036 1.602 1.647 0.045 1.757 1.840 0.083 1.730 1.789 0.050 Figure 4 Representation surfaces in which the radius of the surface is proportional to the size of the effect. Red indicates negative signs. 3 CREATED USING THE RSC ARTICLE TEMPLATE - SEE HTTP://WWW.RSC.ORG/IS/JOURNALS/TEMPLATES/TEMPLATES.HTM FOR FURTHER DETAILS Optical Rotation When employing the theory as outlined above we found a variation of the optical rotation contrary to intuition based solely on atomic polarizabilities. The calculated values of optical rotation for Ph4C, -Si, -Ge, -Sn and -Pb are 252, 32, -33, -75 and -40°/mm, respectively (Figure 5). Unexpectedly, the optical rotation rose sharply on going from the polarizable tin derivative to the least polarizable tetraphenylmethane. Figure 7 Calculated anisotropic electronic polarizabilities in Ph4X. Three hydrogen polarizabilities diverged, an unavoidable consequence of fitting the experimental refractive indices. For optical rotation, we venture a structural interpretation. In the propeller shaped Ph4X molecules one can identify at least two different helical circuits of closely bonded atoms when looking toward the a axis (Figure 6). The sense of rotation opposes the helix if the maximum of the anisotropic polarizability volumes point towards the helix axis whereas the sense of rotation follows the helix when the polarizability volumes are tangential.18 It appears that there is a competition between the two helices, 1-2-3-4-5 and A-B-C-D. The helix 1-2-3-4-5 that defines the general disposition of the phenyl rings produces dextrorotation. However, this “aromatic” optical rotation is counterbalanced by the increasing levorotation of A-B-C-D, which increases with αX. In all compounds, except Ph4C, the polarizability volume of the phenyl carbon coordinated to the central atom (C2) was oriented radially, or towards the helix axis (Figure 7). Thus for Ph4C, A-B-C-D cannot counterbalance 1-2-3-4-5. As shown in Figure 5, the optical rotation reaches a minimum for Ph4Sn and begins to rise again for Ph4Pb. Nevertheless, the X-C2 bond increases throughout the series reaching a maximum length at Ph4Pb, and thereby mitigates the opposing levorotatory influence of helix AB-C-D. Thus, the optical rotation begins again to rise. We also observed that the dihedral angle between phenyl groups γ (Figure 6) was correlated with optical rotation. The larger the value of γ, the stronger the positive contribution of that helix. In fact, the torsion angle C1-C2-C4-C5 (approximated by β-γ) followed the trend of optical rotation (Table 2, Figure 5). Figure 5 Calculated optical rotation plotted against the polarizability of X in Ph4X. We attempted to confirm the expectation for large optical rotations in the Ph4X family with point symmetries42m(D2d). Generally, however, measurements of chiro-optical properties such as optical rotation are thwarted by the much larger birefringence. We therefore had to resort to special polarimetric techniques.17 In this way we confirmed that Ph4Sn was levorotatory along the absolute a direction determined on the basis of anomalous X-ray diffraction according to the coordinates given in Appendix 2. The error remains large because of scattering from the very soft, hard-to-polish surfaces. Small crystallites of Ph4C only extinguished with the polarizer and analyzer nearly parallel. This indicates a huge optical rotation in Ph4C, which is predicted in our calculation. Induced Optical Properties The induced effects in each group increase by and large with increasing polarizability in accordance with the DES model, which predicts larger effects for larger polarizability differences. It is interesting to note how the calculated electro-optic phenomena compare with commonly used materials. The values estimated for electrogyration in Ph4Pb and Ph4Sn reach far above the largest value reliably observed in a solid crystalline material, 0.1×10-5 o/V (normalized by the dielectric constant) in Pb(NO3)2 along [111].19 The d-coefficients are characterized by the figure of merit (d2n-3). Ph4Sn gives here a value of 1.07(pm/V)2. This is to be compared with KH2PO4,20 0.045(pm/V)2 and the best known material, β-bariumborate, 56(pm/V)2. Newkirk cites a personal communication with Bölger and Jerphagnon concerning the d-coefficients, which are in the range of KH2PO4.16 The calculated values for the electrooptic effect are remarkable. With expected values of the relative dielectric constants for the Ph4X series of 5-15, the calculated electro-optic effect exceeds that in KH2PO4 by at least a factor of 10. Newkirk also reported a large r123 of about 17±1pm/V with a relative dielectric constant of about 10; neither the particular compounds measured Figure 6 Helical circuits of closely bonded atoms in Ph4X, 1-2-3-4-5 (atoms polarized tangentially) and A-B-C-D (atoms polarized radially, except for Ph4C), and angles. Projection is normal to (100). 4 CREATED USING THE RSC ARTICLE TEMPLATE - SEE HTTP://WWW.RSC.ORG/IS/JOURNALS/TEMPLATES/TEMPLATES.HTM FOR FURTHER DETAILS nor the variation within the series was specified.16 Yet, our calculated values were 2 to 5 times larger (Table 2). over the face-normal vector h, the term h = (000) should be omitted.1 Alternative Determination of Electronic Polarizability Appendix 2 If the estimated polarizabilities chosen to best match experimentally determined indices of refraction have realistic values, is there a way to determine them based on experiment? In general, the electronic polarizability should be in proportion to the atomic electron densities. The same is true for the x-ray scattering factors. By using the peak heights in the Fourier maps derived for structure solutions, which represent the electron densities at atoms Structure Coordinates of Ph4Sn we hoped to find a correlation between these peak heights and the polarizabilities that were found by comparing the calculated and experimental refractive indices. The peak heights are not absolute but can be normalized to a common atom, i.e. the phenyl carbon atoms. The selection of electronic polarizabilities αX, fractions of peak heights, and values obtained by multiplying the fractions with the polarizability of carbon (αC=0.58Å3) are shown in Table 3. H C Si Ge Sn Pb PX/PC αX=αC PX/PC α X (Å3, Table 2) 0.12 0.070 0.060 1.1 0.61 0.62 4.0 2.3 4.5 11 6.4 5.0 16 9.3 8.8 18 10 9.5 † γ + R3 4πε 0 1 QSS ' = − − S' R3 ∑l ' H αβ ( RrSSl ' ' ) + δ αβ δ SS ' 3ε π π 0 1 ε 0νR 2 R3 2πε 0 ∑h ' hα hβ Ge ih (r −r ) + S 2 ∑h '[(hα δ βγ + hβ δ αγ ) + R 2 hα hβ hγ G' e ih (r −r ) ] − S S' ∑ H αβ (RrSSl ' ' )rSSl ' ' l' exp(− h 2 / R 2 ) G= , G ' = ∂G / ∂k γ , h2 / R2 xα x β H αβ (x) = 2 ψ (| x |) − δ αβ Φ (| x |), x ψ (| x |) = 3Φ (| x |) + 4e −| x| π 2 2 ,Φ (| x |) = Sn C2 C3 C4 C5 C6 C7 0 -0.0189(2) 0.0539(3) 0.0424(4) -0.0419(4) -0.1159(4) -0.1043(4) 0 0.1451(3) 0.2333(3) 0.3265(3) 0.3342(3) 0.2479(3) 0.1540(4) 0 0.1853(4) 0.1674(5) 0.2876(6) 0.4257(6) 0.4454(6) 0.3264(7) Supplementary information on the crystal structures has been deposited and can be obtained free of charge from the publisher. 1 V. Devarajan and A. M. Glazer, Acta Crystallogr. Sect A., 1986, 42, 560. 2 G. Beurskens-Kerssen, J. Kroon, H. J. Endemann, J. van Laar and J. M. Bijvoet, in Crystallography and Crystal Perfection, ed. G. Ramachandran, Academic Press, London, 1963, p. 225; J. M. Bijvoet, A. F. Peerdeman and A. J. Van Bomel, Nature, 1951, 168, 271; M. Born and M. Goeppert-Mayer, in Handbuch der Physik, 1933, 24, 623; G. Bruhat and P. Grivet, J. Phys. Radium, 1935, 6, 12; J. van Laar, H. J. Endemann and J. M. Bijvoet, Acta Crystallogr. Sect. A., 1968, 24, 52; R. Reijnhart, PhD thesis, Delft, 1970. 3 J. D. Jackson, Classical Electrodynamics, Second Edition, John Wiley & Sons, New York, 1975, p. 220. 4 P. P. Ewald, Ann. Phys., 1921, 64, 253. 5 W. Kaminsky and A. M. Glazer, Z. Kristallogr., 1997, 212, 283. 6 W. Kaminsky and A. M. Glazer, Phase Transitions, 1997, 66, 1. 7 R. K. Kondru, P. Wipf, and D. N. Beratan, Science, 1998, 282, 2247. 8 C. Kittel, Introduction to Solid State Physics, Fifth Edition, John Wiley & Sons, Inc., New York, 1976, p. 399. 9 J. R. Tessman, A. H. Kahn and W. Shokley, Phys. Rev., 1953. 92, 891. 10 N. W. Ashcroft and N. D. Mermin, Solid State Physics, Holt, Rinehart and Winston, London, 1976, p. 546. 11 L. Bohatý, Z. Kristallogr, 1984, 166, 97. 12 D. A. Kleinmann, Phys. Rev., 1962, 128, 133. 13 A. Robbins, G. A. Jeffrey, J. P. Chesick, J. Donohue, F. A. Cotton, B. A. Frenz and C. A. Murillo, Acta Crystallor. Sect. B., 1975, B31, 2395; V. Gruhnert, A. Kirfel, G. Will, F. Wallrafen and K. Recker, Z. Kristallogr., 1983, 163, 53; A. Karipides and D. A. Haller, Acta Crystallogr. Sect. B., 1972, B28, 2889; P. C. Chieh and J. Trotter, J. Chem. Soc., 1970, 911; V. Busetti, M. Mammi, A. Signor and A. Del Pra, Inorg. Chim. Acta., 1967, 1, 424. 14 M. A. Lloyd and C. P. Brock, Acta Crystallogr., Sect. B, 1997, B53, 780. 15 N. H. Hartshorne and A. Stuart, Practical Optical Crystallography, Edward Arnold Publishers, London, 1964, p. 230. 16 H. W. Newkirk, J. Organomet. Chem., 1972, 44, 269. 17 W. Kaminsky and A. M. Glazer, Ferroelectrics, 1996, 183, 133; J. Kobayashi and Y. Uesu, J. Appl. Crystallogr., 1983, 16, 204. 18 A. M. Glazer and K. Stadnicka, J. Appl. Crystallogr., 1986, 19, 108. 19 H. J. Weber and S. Haussühl, Z. Kristallogr., 1977, 146, 3030; W. Kaminsky, A. Fahnenstich and S. Haussuehl, Ann. Phys., 1992, 1, 92. 20 J. Jerphagnon and S. K. Kurtz, Phys. Rev., 1970, B1, 1749. 21 G. A. Ivanov – Smolenskii, V. G. Tsirelson, and R. P. Ozerov, Acta Crystallogr., 1983, A39, 411. 0 1 QSS ' = QSS ' + i ∑ QSS ' kγ Q z/c References Appendix 1 1 =− ε 0νR 2 y/b We are grateful to Prof. S. Haussühl for donating tetraphenylsilane crystals and for financial support from the Petroleum Research Fund of the American Chemical Society (35706-AC06) and from the National Science Foundation (CHE-0092617). For previous attempts to calculate electronic polarizabilities from X-ray structure amplitudes see Ivanov – Smolenskii et al.21 Surprisingly, we found a relatively large polarizability for aromatic hydrogen atoms derived from both estimated refractive indices and the Fourier maps. 0 SS ' x/a Acknowledgements Table 3 Electron density and electronic polarizability. PX/PC is the ratio of Fourier peak heights of atom X and the aromatic carbon, and αX is the polarizability of atom X. X= Atom 1 2e −|x| erfc (| |) , x + | x |3 π l' l' rSS ' = r + rS ' − rS Indices α, β and γ refer to a Cartesian reference system and R is a parameter chosen so as to ensure convergence. The term corresponding to unit cell index l’=0 with S=S’ is ignored in the summation over l’. In the summation 5 CREATED USING THE RSC ARTICLE TEMPLATE - SEE HTTP://WWW.RSC.ORG/IS/JOURNALS/TEMPLATES/TEMPLATES.HTM FOR FURTHER DETAILS 6